DOI: 10.17188/1475717
title: Materials Data on Sr2Ca2Co3CuO10 by Materials Project

description: Sr2Ca2Co3CuO10 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are sixteen inequivalent Sr2+ sites. In the first Sr2+ site, Sr2+ is bonded in a 10-coordinate geometry to ten O2- atoms. There are a spread of Sr–O bond distances ranging from 2.49–3.19 Å. In the second Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–3.02 Å. In the third Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.50–2.87 Å. In the fourth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.16 Å. In the fifth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.02 Å. In the sixth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.11 Å. In the seventh Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–2.99 Å. In the eighth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.39–2.79 Å. In the ninth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.04 Å. In the tenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.51–2.96 Å. In the eleventh Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.50–2.91 Å. In the twelfth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.43–2.77 Å. In the thirteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.03 Å. In the fourteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.15 Å. In the fifteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.14 Å. In the sixteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.03 Å. There are sixteen inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.94 Å. In the second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.98 Å. In the third Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.95 Å. In the fourth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.25–2.58 Å. In the fifth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.28–2.87 Å. In the sixth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.65 Å. In the seventh Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.87 Å. In the eighth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.80 Å. In the ninth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.26–2.94 Å. In the tenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.28–2.71 Å. In the eleventh Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.27–2.59 Å. In the twelfth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.26–2.63 Å. In the thirteenth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.66 Å. In the fourteenth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.67 Å. In the fifteenth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.59 Å. In the sixteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.29–2.93 Å. There are twenty-four inequivalent Co+3.33+ sites. In the first Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–11°. There are a spread of Co–O bond distances ranging from 1.82–2.20 Å. In the second Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form distorted CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 1–13°. There are a spread of Co–O bond distances ranging from 1.83–2.46 Å. In the third Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 6–14°. There are a spread of Co–O bond distances ranging from 1.83–2.17 Å. In the fourth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 4–13°. There are a spread of Co–O bond distances ranging from 1.84–2.29 Å. In the fifth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 trigonal pyramid. The corner-sharing octahedra tilt angles range from 8–12°. There are a spread of Co–O bond distances ranging from 1.84–2.18 Å. In the sixth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form distorted CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 2–13°. There are a spread of Co–O bond distances ranging from 1.86–2.52 Å. In the seventh Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 trigonal pyramid. The corner-sharing octahedra tilt angles range from 7–13°. There are a spread of Co–O bond distances ranging from 1.84–2.19 Å. In the eighth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 1–12°. There are a spread of Co–O bond distances ranging from 1.83–2.37 Å. In the ninth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–14°. There are a spread of Co–O bond distances ranging from 1.87–2.23 Å. In the tenth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 trigonal pyramid. The corner-sharing octahedra tilt angles range from 3–13°. There are a spread of Co–O bond distances ranging from 1.86–2.33 Å. In the eleventh Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–12°. There are a spread of Co–O bond distances ranging from 1.86–2.10 Å. In the twelfth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form distorted CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 trigonal pyramid. The corner-sharing octahedra tilt angles range from 6–13°. There are a spread of Co–O bond distances ranging from 1.81–2.43 Å. In the thirteenth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form distorted CoO6 octahedra that share corners with four CoO6 octahedra and corners with two CoO4 tetrahedra. The corner-sharing octahedra tilt angles range from 6–12°. There are a spread of Co–O bond distances ranging from 1.81–2.55 Å. In the fourteenth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 1–9°. There are a spread of Co–O bond distances ranging from 1.89–2.35 Å. In the fifteenth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–12°. There are a spread of Co–O bond distances ranging from 1.82–2.15 Å. In the sixteenth Co+3.33+ site, Co+3.33+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 1–12°. There are a spread of Co–O bond distances ranging from 1.80–2.33 Å. In the seventeenth Co+3.33+ site, Co+3.33+ is bonded to four O2- atoms to form CoO4 tetrahedra that share corners with two CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 27–38°. There are a spread of Co–O bond distances ranging from 1.81–1.93 Å. In the eighteenth Co+3.33+ site, Co+3.33+ is bonded to four O2- atoms to form CoO4 tetrahedra that share corners with two CoO6 octahedra and corners with two CoO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–34°. There are a spread of Co–O bond distances ranging from 1.81–1.98 Å. In the nineteenth Co+3.33+ site, Co+3.33+ is bonded to four O2- atoms to form CoO4 tetrahedra that share corners with two CoO6 octahedra, a cornercorner with one CoO4 tetrahedra, and a cornercorner with one CuO4 tetrahedra. The corner-sharing octahedra tilt angles range from 22–39°. There are a spread of Co–O bond distances ranging from 1.81–1.93 Å. In the twentieth Co+3.33+ site, Co+3.33+ is bonded to four O2- atoms to form CoO4 tetrahedra that share corners with two CoO6 octahedra, a cornercorner with one CuO4 tetrahedra, and a cornercorner with one CuO4 trigonal pyramid. The corner-